Preparation and Characterization of Thermo-Responsive Rod-Coil Diblock Copolymers

In this study, we synthesized amphiphilic poly(2,7–(9,9–dioctylfluorene))–block–N,N–(diisopropylamino)ethyl methacrylate (POF–b–PDPMAEMA) rod-coil diblock copolymers by atom transfer radical polymerization (ATRP). The structure and multifunctional sensing properties of these copolymers were also investigated. The POF rod segment length of 10 was fixed and the PDPAEMA coil segment lengths of 90 and 197 were changed, respectively. The micellar aggregates of POF10–b–PDPAEMA90 rod-coil diblock copolymer in water showed a reversible shape transition from cylinder bundles to spheres when the temperature was changed from 20 to 80 °C or the pH was changed from 11 to 2. The atomic force microscopy (AFM) and transmission electron microscopy (TEM) measurements indicated that the temperature had also an obvious influence on the micelle size. In addition, since POF10–b–PDPAEMA90 had a lower critical solution temperature, its photoluminescence (PL) intensity in water is thermoreversible. The PL spectra showed that the POF–b–PDPAEMA copolymer had a reversible on/off profile at elevated temperatures, and thus could be used as an on/off fluorescent indicator for temperature or pH. The fluorescence intensity distribution of pH switched from “off–on” to “on–off” as the temperature increased. These results showed that the POF–b–PDPAEMA copolymer has a potential application for temperature and pH sensing materials.


Introduction
The self-assembly of conjugated rod-coil block copolymers has been studied extensively towards novel structural, functional, and physical properties of supramolecular species [1][2][3]. The aggregation and microphase separation of such block copolymers driven by various novel functionalities of p-p interaction through solvent selection or rigid segmentation may result in various nanosized morphologies [4][5][6]. Different conjugated rod-coil block copolymers have been reported in the literature, including those of thiophene [7,8], phenylene [9][10][11], and quinolone [12,13]. The fluorene-based rod-coil block copolymers were used in this study because of their high thermal/chemical stability and good fluorescence quantum yield [14][15][16]. Incorporating the coil segment into the backbone not only allows the possibility to control the electronic and optoelectronic properties, but also produces self-assembled nanostructures, such as spheres, worms, honeycombs, or linear structures [17]. Besides, the combination of the stimulus-responsive coil section and the tunable photophysical properties will result in novel multifunctional sensing materials [18,19]. Recently, the
The chemical structure of synthesized copolymers was confirmed by Fourier transform infrared (FTIR) spectra (PerkinElmer Spectrum spectrophotometer, Waltham, MA, USA) and NMR spectra Polymers 2017, 9, 340 3 of 10 (Jeol EX-400 spectrometer, Tokyo, Japan). The photophysical properties of copolymer films were tested by ultraviolet-visible spectrophotometry (Jasco Model V-650, Oklahoma, OK, USA) and photoluminescence spectroscopy (Horiba Jobin Yvon Fluoromax-4 Spectro fluorometer, Tokyo, Japan). The adsorption spectra were measured in the range of 200-800 nm and an excitation wavelength of 450 nm was used in emission spectrum. Gel permeation chromatography calibrated by 0.5 wt % PS standard in THF with a flowrate of 1 mL/min at 40 • C was used to measure the molecular weight distribution of copolymers. A refractive index detector (Schambeck SFD GmbH, model RI 2000, Bad Honnef, Germany) with a PLgel 5 µm mixed-C and D column were used in gel permeation chromatography. Surface structure of copolymers were examined by a transmission electron microscopy (JEOL 1210) and atomic force microscope (Bruker Nanoscope DI III multimode AFM, Billerica, MA, USA) measurements under an acceleration voltage of 100 kV and a tapping mode, respectively. Figure 1 illustrates the variation of optical transmittance with temperature for the prepared copolymers, POF 10 -b-PDPAEMA 197 and POF 10 -b-PDPAEMA 90 . It shows that the copolymer with a longer PDEAEMA chain length had a high transmission because of favorable solubility in water. In addition, the copolymer exhibited a lower critical solution temperatures (LCST) of 40 • C. At this temperature, the optical transmission of the copolymer solution decreased, because the micelle structure of copolymers aggregated, leading to reduced transmittance. The optical transmittance decreased as the chain length of the DPAEMA segment increased. Therefore, the reduction of optical transmittance for POF 10 -b-PDPAEMA 197 was more apparent than that obtained from POF 10 -b-PDPAEMA 90 .

Results and Discussion
Polymers 2017, 9,340 3 of 10 (Jeol EX-400 spectrometer, Tokyo, Japan). The photophysical properties of copolymer films were tested by ultraviolet-visible spectrophotometry (Jasco Model V-650, Oklahoma, OK, USA) and photoluminescence spectroscopy (Horiba Jobin Yvon Fluoromax-4 Spectro fluorometer, Tokyo, Japan). The adsorption spectra were measured in the range of 200-800 nm and an excitation wavelength of 450 nm was used in emission spectrum. Gel permeation chromatography calibrated by 0.5 wt % PS standard in THF with a flowrate of 1 mL/min at 40 °C was used to measure the molecular weight distribution of copolymers. A refractive index detector (Schambeck SFD GmbH, model RI 2000, Bad Honnef, Germany) with a PLgel 5 μm mixed-C and D column were used in gel permeation chromatography. Surface structure of copolymers were examined by a transmission electron microscopy (JEOL 1210) and atomic force microscope (Bruker Nanoscope DI III multimode AFM, Billerica, MA, USA) measurements under an acceleration voltage of 100 kV and a tapping mode, respectively. Figure 1 illustrates the variation of optical transmittance with temperature for the prepared copolymers, POF10-b-PDPAEMA197 and POF10-b-PDPAEMA90. It shows that the copolymer with a longer PDEAEMA chain length had a high transmission because of favorable solubility in water. In addition, the copolymer exhibited a lower critical solution temperatures (LCST) of 40 °C. At this temperature, the optical transmission of the copolymer solution decreased, because the micelle structure of copolymers aggregated, leading to reduced transmittance. The optical transmittance decreased as the chain length of the DPAEMA segment increased. Therefore, the reduction of optical transmittance for POF10-b-PDPAEMA197 was more apparent than that obtained from POF10-b-PDPAEMA90.  Such a thermo-responsive behaviors of copolymers have been reported [33]. The temperaturesensitive segment of PF10-b-PDPAEMA197 is longer, so its shape changes rapidly as the temperature    Figure 3 illustrates the PL intensity of POF10-b-PDPAEMA90 in water when it was subjected to a heating and cooling cycle between 30 and 80 °C. It shows that the PL intensity decreased at the heating stage and increased again at the cooling stage. The formation of intramolecular hydrogen bonding between PDPAEMA chains results in this thermo-responsive phenomenon. Heating the solution above the LCST (40 °C) caused the intramolecular hydrogen bonding of the PDPAEMA and the structure formed closely packed aggregates that resulted in the reduction of PL intensity [24,33]. On the contrary, cooling the solution below the LCST led to a swelling of the PDPAEMA corona in water. Consequently, the POF core can absorb more incident light and increases the light emission intensity. Figure 4 illustrates the PL intensity of POF10-b-PDPAEMA197 in water when it was subjected to a heating and cooling cycle between 30 and 80 °C. Comparing Figures 3 and 4 shows that the change of fluorescence intensity for POF10-b-PDPAEMA197 is significantly faster than POF10-b-PDPAEMA90, because POF10-b-PDPAEMA197 has longer thermo-responsive chain lengths that caused a faster aggregation of micelles and thus the apparent change in photoluminescence.  Such a thermo-responsive behaviors of copolymers have been reported [33]. The temperaturesensitive segment of PF 10 -b-PDPAEMA 197 is longer, so its shape changes rapidly as the temperature changes, resulting in a larger slope of the change in optical transmittance and thus a narrower loop width than the PF 10 -b-PDPAEMA 90 [34]. Figure 3 illustrates the PL intensity of POF 10 -b-PDPAEMA 90 in water when it was subjected to a heating and cooling cycle between 30 and 80 • C. It shows that the PL intensity decreased at the heating stage and increased again at the cooling stage. The formation of intramolecular hydrogen bonding between PDPAEMA chains results in this thermo-responsive phenomenon. Heating the solution above the LCST (40 • C) caused the intramolecular hydrogen bonding of the PDPAEMA and the structure formed closely packed aggregates that resulted in the reduction of PL intensity [24,33]. On the contrary, cooling the solution below the LCST led to a swelling of the PDPAEMA corona in water. Consequently, the POF core can absorb more incident light and increases the light emission intensity. changes, resulting in a larger slope of the change in optical transmittance and thus a narrower loop width than the PF10-b-PDPAEMA90 [34].  Figure 3 illustrates the PL intensity of POF10-b-PDPAEMA90 in water when it was subjected to a heating and cooling cycle between 30 and 80 °C. It shows that the PL intensity decreased at the heating stage and increased again at the cooling stage. The formation of intramolecular hydrogen bonding between PDPAEMA chains results in this thermo-responsive phenomenon. Heating the solution above the LCST (40 °C) caused the intramolecular hydrogen bonding of the PDPAEMA and the structure formed closely packed aggregates that resulted in the reduction of PL intensity [24,33]. On the contrary, cooling the solution below the LCST led to a swelling of the PDPAEMA corona in water. Consequently, the POF core can absorb more incident light and increases the light emission intensity. Figure 4 illustrates the PL intensity of POF10-b-PDPAEMA197 in water when it was subjected to a heating and cooling cycle between 30 and 80 °C. Comparing Figures 3 and 4 shows that the change of fluorescence intensity for POF10-b-PDPAEMA197 is significantly faster than POF10-b-PDPAEMA90, because POF10-b-PDPAEMA197 has longer thermo-responsive chain lengths that caused a faster aggregation of micelles and thus the apparent change in photoluminescence.    Figure 5 illustrates the variation in the surface structures for the POF10-b-PDPAEMA90 in water with temperature. It shows that the surface structure consisted of cylinder bundles at 30 °C (below the LCST), but changed to cylinders at 50 °C (above the LCST). However, the surface structure exhibited spheres at 60 °C, and the spheres aggregated at 80 °C. The described structural change of the micelles can be attributed to the variation in the hydrophilic/hydrophobic property of PDEAEMA. The highly hydrophilic PDPAEMA block showed an extended corona conformation as the temperature was below its LCST. However, as the temperature was raised above the LCST, the formation of intramolecular hydrogen bonding between the PDPAEMA chains caused a closely packed arrangement, thus water molecules were excluded from the corona. Therefore, the radius of cylindrical micelles became smaller. Nevertheless, increasing the temperature from 60 to 80 °C could enhance the intramolecular hydrogen bonding of the corona; thus, the corona became highly contracted, disrupting the POF aggregation. Figure 6 shows the  Figure 5 illustrates the variation in the surface structures for the POF 10 -b-PDPAEMA 90 in water with temperature. It shows that the surface structure consisted of cylinder bundles at 30 • C (below the LCST), but changed to cylinders at 50 • C (above the LCST). However, the surface structure exhibited spheres at 60 • C, and the spheres aggregated at 80 • C. The described structural change of the micelles can be attributed to the variation in the hydrophilic/hydrophobic property of PDEAEMA. The highly hydrophilic PDPAEMA block showed an extended corona conformation as the temperature was below its LCST. However, as the temperature was raised above the LCST, the formation of intramolecular hydrogen bonding between the PDPAEMA chains caused a closely packed arrangement, thus water molecules were excluded from the corona.  Figure 5 illustrates the variation in the surface structures for the POF10-b-PDPAEMA90 in water with temperature. It shows that the surface structure consisted of cylinder bundles at 30 °C (below the LCST), but changed to cylinders at 50 °C (above the LCST). However, the surface structure exhibited spheres at 60 °C, and the spheres aggregated at 80 °C. The described structural change of the micelles can be attributed to the variation in the hydrophilic/hydrophobic property of PDEAEMA. The highly hydrophilic PDPAEMA block showed an extended corona conformation as the temperature was below its LCST. However, as the temperature was raised above the LCST, the formation of intramolecular hydrogen bonding between the PDPAEMA chains caused a closely packed arrangement, thus water molecules were excluded from the corona. Therefore, the radius of cylindrical micelles became smaller. Nevertheless, increasing the temperature from 60 to 80 °C could enhance the intramolecular hydrogen bonding of the corona; thus, the corona became highly contracted, disrupting the POF aggregation. Figure 6 shows the Therefore, the radius of cylindrical micelles became smaller. Nevertheless, increasing the temperature from 60 to 80 • C could enhance the intramolecular hydrogen bonding of the corona; thus, the corona became highly contracted, disrupting the POF aggregation. Figure 6 shows the variation in the surface structures for the POF  in water with temperature. The surface structure consisted of cylinder bundles at 30 • C, but changed to spheres at 50 • C (above the LCST) because of the longer chain length of the hydrophobic PDPAEMA segment [35]. Aggregates of spherical micelles were observed at higher temperatures (60-80 • C) because the long hydrophobic segment reduced the colloidal stability in water, resulting in larger interconnected micelles, as shown in Figure 6c,d.

Results and Discussion
Polymers 2017, 9, 340 6 of 10 variation in the surface structures for the POF10-b-PDPAEMA197 in water with temperature. The surface structure consisted of cylinder bundles at 30 °C, but changed to spheres at 50 °C (above the LCST) because of the longer chain length of the hydrophobic PDPAEMA segment [35]. Aggregates of spherical micelles were observed at higher temperatures (60-80 °C) because the long hydrophobic segment reduced the colloidal stability in water, resulting in larger interconnected micelles, as shown in Figure 6c,d.  Figure 7 illustrates the PL spectra of POF10-b-PDPAEMA90 in water at different solution pH. It can be seen that the PL intensity was weak at acidic pH, but strengthened as the pH increased from pH = 2 to 9. Over pH = 9, the PL intensity decreased again with increasing pH. This is because the PDPAEMA chains at acidic pH led to the formation of large polymer spheres so that scarcely any incident light was absorbed by the POF core, resulting in weak emission intensity. In addition, the pH-sensitive PDPAEMA segment undergoes a decrease in the conjugate plane resulting from the aggregation of the deprotonated chains in the high pH environment, resulting in a decrease in the fluorescence intensity [36,37]. Figure 8 illustrates the PL intensity of POF10-b-PDPAEMA90 and POF10-b-PDPAEMA197 in water at different solution pH. It shows that the PL intensity of POF10-b-PDPAEMA197 decreased at lower pH levels (pH = 7) than that (pH = 9) of POF10-b-PDPAEMA90, because the copolymer with a longer PDPMAEMA segment more readily undergoes aggregation at lower pH levels.  Figure 7 illustrates the PL spectra of POF 10 -b-PDPAEMA 90 in water at different solution pH. It can be seen that the PL intensity was weak at acidic pH, but strengthened as the pH increased from pH = 2 to 9. Over pH = 9, the PL intensity decreased again with increasing pH. This is because the PDPAEMA chains at acidic pH led to the formation of large polymer spheres so that scarcely any incident light was absorbed by the POF core, resulting in weak emission intensity. In addition, the pH-sensitive PDPAEMA segment undergoes a decrease in the conjugate plane resulting from the aggregation of the deprotonated chains in the high pH environment, resulting in a decrease in the fluorescence intensity [36,37]. Figure 8 illustrates the PL intensity of POF 10 -b-PDPAEMA 90 and POF  in water at different solution pH. It shows that the PL intensity of POF 10 -b-PDPAEMA 197 decreased at lower pH levels (pH = 7) than that (pH = 9) of POF 10 -b-PDPAEMA 90 , because the copolymer with a longer PDPMAEMA segment more readily undergoes aggregation at lower pH levels.  Figures 9 and 10 illustrate the TEM images of the POF10-b-PDPAEMA90 and POF10-b-PDPAEMA197 micellar aggregates to show the structural change induced by pH variation. It shows that the spherical small micelles were observed at pH = 2, as shown in Figure 9a. As the pH increased to 7, the cylinder bundles were observed as shown in Figure 9b due to the interaction between the PDPAEMA and the POF π-π bond at both ends of the POF, the PDPAEMA is deprotonated and induces the aggregation, resulting in the transformation of the structure into shorter and coarse cylindrical micelles. As the pH value continues to rise, its morphology is transformed into a single monoclinic micelle, because the increase in the pH value suppresses the electrostatic repulsion of PDPAEMA, and the diameter becomes smaller into a thin cylindrical micelle as shown in Figure 9c. The result indicates that the pH value controls the degree of charge in the corona of the PDPAEMA block and induces swelling or shrinking because of the electrostatic repulsion. It means that the addition or removal of a proton (H) to or from PDPAEMA has an obvious influence on the copolymer structure. As shown in Figure 10, the POF10-b-PDPAEMA197 copolymers show a similar structural transformation.  Figures 9 and 10 illustrate the TEM images of the POF10-b-PDPAEMA90 and POF10-b-PDPAEMA197 micellar aggregates to show the structural change induced by pH variation. It shows that the spherical small micelles were observed at pH = 2, as shown in Figure 9a. As the pH increased to 7, the cylinder bundles were observed as shown in Figure 9b due to the interaction between the PDPAEMA and the POF π-π bond at both ends of the POF, the PDPAEMA is deprotonated and induces the aggregation, resulting in the transformation of the structure into shorter and coarse cylindrical micelles. As the pH value continues to rise, its morphology is transformed into a single monoclinic micelle, because the increase in the pH value suppresses the electrostatic repulsion of PDPAEMA, and the diameter becomes smaller into a thin cylindrical micelle as shown in Figure 9c. The result indicates that the pH value controls the degree of charge in the corona of the PDPAEMA block and induces swelling or shrinking because of the electrostatic repulsion. It means that the addition or removal of a proton (H) to or from PDPAEMA has an obvious influence on the copolymer structure. As shown in Figure 10, the POF10-b-PDPAEMA197 copolymers show a similar structural transformation. Figures 9 and 10 illustrate the TEM images of the POF 10 -b-PDPAEMA 90 and POF 10 -b-PDPAEMA 197 micellar aggregates to show the structural change induced by pH variation. It shows that the spherical small micelles were observed at pH = 2, as shown in Figure 9a. As the pH increased to 7, the cylinder bundles were observed as shown in Figure 9b due to the interaction between the PDPAEMA and the POF π-π bond at both ends of the POF, the PDPAEMA is deprotonated and induces the aggregation, resulting in the transformation of the structure into shorter and coarse cylindrical micelles. As the pH value continues to rise, its morphology is transformed into a single monoclinic micelle, because the increase in the pH value suppresses the electrostatic repulsion of PDPAEMA, and the diameter becomes smaller into a thin cylindrical micelle as shown in Figure 9c. The result indicates that the pH value controls the degree of charge in the corona of the PDPAEMA block and induces swelling or shrinking because of the electrostatic repulsion. It means that the addition or removal of a proton (H) to or from PDPAEMA has an obvious influence on the copolymer structure. As shown in Figure 10, the POF 10 -b-PDPAEMA 197 copolymers show a similar structural transformation.

Conclusions
In this study, we have synthesized the POF-b-PDPAEMA rod-coil block copolymers that show a significant variation in their surface structure and photophysical properties with respect to the temperature and pH. The micellar aggregates of POF10-b-PDPAEMA90 in water show a reversible change of surface structure from cylinder bundles to spheres under a heating-cooling cycle of 30-80 °C. The LCST of POF10-b-PDMAEMA90 decreased with an increase in solution pH values due to the deprotonation of the PDPAEMA block. On the other hand, the light emission intensity for POF10-b-PDPAEMA90 in water was thermo-responsive, depending on its lower critical solution temperatures. It means that the prepared copolymers in this study can be applied as on/off fluorescence indicators and thus as temperature and acid-base value sensory materials, since the POF-b-PDPAEMA copolymer shows a stable and reversible ''on-off'' profile.

Conclusions
In this study, we have synthesized the POF-b-PDPAEMA rod-coil block copolymers that show a significant variation in their surface structure and photophysical properties with respect to the temperature and pH. The micellar aggregates of POF10-b-PDPAEMA90 in water show a reversible change of surface structure from cylinder bundles to spheres under a heating-cooling cycle of 30-80 °C. The LCST of POF10-b-PDMAEMA90 decreased with an increase in solution pH values due to the deprotonation of the PDPAEMA block. On the other hand, the light emission intensity for POF10-b-PDPAEMA90 in water was thermo-responsive, depending on its lower critical solution temperatures. It means that the prepared copolymers in this study can be applied as on/off fluorescence indicators and thus as temperature and acid-base value sensory materials, since the POF-b-PDPAEMA copolymer shows a stable and reversible ''on-off'' profile.